Pb(II) Adsorption by a Calcium Metal-Organic Framework †

: Among the water pollution sources, heavy metals are considered the most hazardous because of their high toxicity to human health and their ability to badly damage the kidneys, brain, and nerves, as well as cause birth defects. Based on the promising features of metal-organic frameworks ( MOFs), they could act as a favorable candidate in heavy metal removal applications. A calcium-based metal-organic framework was synthesized by the deposition method using benzene-1,2,4,5-tetracarboxylate as a linker. After characterization of the MOF was performed using X-ray Diffraction (XRD), Scanning Electron Microscopy (SEM) and Fourier Transform Infrared (FTIR) analyses, it was applied to efﬁcient adsorption of Pb(II) pollutant ions. The potential of obtained MOF, [Ca(H 2 btec) · H 2 O] n , H 2 btec: benzene-1,2,4,5-tetracarboxylic acid was investigated by adsorbing Pb(II) ions in an aqueous solution, separating the adsorbent using centrifugation, and ﬁnally measuring the residual Pb(II) ions using the ICP-AES method.


Introduction
With developing industrial efforts, decreasing clean water, and increasing water pollution, toxic pollution agents have become an essential problem facing human beings. Wastewaters now contain inorganic chemicals, such as heavy metals, which easily pollute the environment. Metals, including lead (Pb), arsenic (As), mercury (Hg), chromium (Cr), nickel (Ni), barium (Ba), cadmium (Cd), cobalt (Co), selenium (Se), and vanadium (V) are poisonous even in ppb (parts per billion). These toxic elements enter food and water, and even items such as toys; they can damage kidneys, the brain, nerves, and the digestive system. The concentration of lead (Pb 2+ ) in water must not surpass ppb in drinking water. Based on experiments using reticulating metal ions and organic carboxylates as linkers, it has been observed that these methods extended them and allowed for the design of structures to provide increased absorption. In this regard, a metal-organic framework (MOF) is attractive due to its exceptional high porosity. Regarding absorption, heavy metals are important, but green synthesis is also valuable. For every material, synthesized H 2 O was used as a solvent, and the green synthesis method was used. The application of such green-based adsorbents could decrease heavy metal ion levels in wastewater [1,2].

Synthesis of Experimental [Ca(H 2 btec)·H 2 O] n
In total, 1 mol (0.255 g) of benzene-1,2,4,5-tetracarboxylic acid (H 2 btec) was dissolved in 20 cc water, then 10 cc ethanol was added and stirred for 2 min at room temperature until absolutely dissolved. Then, 2 mol (0.47 g) Ca(NO 3 ) 2 was dissolved in 10 cc water, and these two solutions were mixed while stirred at 100 • C, 600 rpm for 2 h, and the resulting solution was cooled to room temperature. The precipitated white powder was dried at room temperature for one day [3].

Pb(II) Ions Adsorption
In this case, the effect of different parameters, such as the effect of Pb(II) initial concentration on the absorbance mass and contact time, were studied. For the isotherm adsorption survey, all the experiments were conducted at room temperature by adding 10 mg of [Ca(H 2 btec)·H 2 O] n to 30 mL of Pb(II) solution with an initial concentration of 12, 25, 50, and 100 mg L −1 . Afterward, the solution was shaken for 15 min at 100 rpm.
The Pb(II) capacity is an important factor that appoints the adsorption capacity for eliminating specific amounts of contaminants. The following Equations (1) and (2) state the contaminant elimination percentage.
In which C 0 (mg L −1 ) and C e (mg L −1 ) are the initial concentration and equivalent concentration of contaminants, respectively. V (mL) is introduced as solution volume, m (g) as adsorbent mass, and q e (mg/g) as surface equivalent adsorption capacity. solution was cooled to room temperature. The precipitated white powder was dried at room temperature for one day [3].

Pb(II) Ions Adsorption
In this case, the effect of different parameters, such as the effect of Pb(II) initial concentration on the absorbance mass and contact time, were studied. For the isotherm adsorption survey, all the experiments were conducted at room temperature by adding 10 mg of [Ca(H2btec)·H2O]n to 30 mL of Pb(II) solution with an initial concentration of 12, 25, 50, and 100 mg L −1 . Afterward, the solution was shaken for 15 min at 100 rpm.
The Pb(II) capacity is an important factor that appoints the adsorption capacity for eliminating specific amounts of contaminants. The following Equations (1) and (2) state the contaminant elimination percentage.
In which C0 (mg L −1 ) and Ce (mg L −1 ) are the initial concentration and equivalent concentration of contaminants, respectively. V (mL) is introduced as solution volume, m (g) as adsorbent mass, and qe (mg/g) as surface equivalent adsorption capacity. Figure 1 shows the XRD pattern of [Ca(H2btec)·H2O]n and exhibits a sharp and highly intense peak at 2θ 26.5°.

FTIR Spectrum
The FTIR spectrum of of [Ca(H2btec)·H2O]n was shown in Figure 2. The bands at 3500 cm −1 and 3650 cm −1 are attributed, respectively, to carboxylic groups and water molecules. The band at 900-690 cm −1 is attributed to the aromatic ring of the linker.

FTIR Spectrum
The FTIR spectrum of of [Ca(H 2 btec)·H 2 O] n was shown in Figure 2. The bands at 3500 cm −1 and 3650 cm −1 are attributed, respectively, to carboxylic groups and water molecules. The band at 900-690 cm −1 is attributed to the aromatic ring of the linker.

Scanning Electron Microscopy
The result shown in Figure 3 illustrates the rod shapes of the MOF particles, with an average size of 1-7 μm.

Effect of pH and Time on Adsorption
The amount of Pb(II) adsorbed onto [Ca(H2btec)·H2O]n is a function of time and pH. As shown in Figure 4, the best pH is 5, in which more than 95% adsorption occurred. Moreover, Pb(II) adsorption is increased to 96% mg g −1 at 15 min, shown in Figure 5 as the highest adsorption and then it remains constant till 35 min.

Scanning Electron Microscopy
The result shown in Figure 3 illustrates the rod shapes of the MOF particles, with an average size of 1-7 µm.

Scanning Electron Microscopy
The result shown in Figure 3 illustrates the rod shapes of the MOF particles, with an average size of 1-7 μm.

Effect of pH and Time on Adsorption
The amount of Pb(II) adsorbed onto [Ca(H2btec)·H2O]n is a function of time and pH. As shown in Figure 4, the best pH is 5, in which more than 95% adsorption occurred. Moreover, Pb(II) adsorption is increased to 96% mg g −1 at 15 min, shown in Figure 5 as the highest adsorption and then it remains constant till 35 min.

Effect of pH and Time on Adsorption
The amount of Pb(II) adsorbed onto [Ca(H 2 btec)·H 2 O] n is a function of time and pH. As shown in Figure 4, the best pH is 5, in which more than 95% adsorption occurred. Moreover, Pb(II) adsorption is increased to 96% mg g −1 at 15 min, shown in Figure 5 as the highest adsorption and then it remains constant till 35 min.

Adsorption of Metallic Ions
On examining toxic metallic ions, including lead, copper, cadmium, chrome, and barium, we found out that the title MOF can adsorb the former most effectively. This can be seen in Figure 6, in which Pb(II) ions are nearly 100% adsorbed, performing much better than the others.

Desorption after Adsorption
After the adsorption of Pb(II), we tried to desorb it from the adsorbent to examine whether the structure of MOF remained or not. Primarily, we searched for lead ions, and, as shown in Figure 7, the Energy-Dispersive X-ray Spectroscopy (EDX). methods results illustrate the presence of the ions in the MOF after adsorption. Afterward, we desorb the ions by removing them from the MOF in D.I. water by washing them in RT three times,

Adsorption of Metallic Ions
On examining toxic metallic ions, including lead, copper, cadmium, chrome, and barium, we found out that the title MOF can adsorb the former most effectively. This can be seen in Figure 6, in which Pb(II) ions are nearly 100% adsorbed, performing much better than the others.

Desorption after Adsorption
After the adsorption of Pb(II), we tried to desorb it from the adsorbent to examine whether the structure of MOF remained or not. Primarily, we searched for lead ions, and, as shown in Figure 7, the Energy-Dispersive X-ray Spectroscopy (EDX). methods results illustrate the presence of the ions in the MOF after adsorption. Afterward, we desorb the ions by removing them from the MOF in D.I. water by washing them in RT three times,

Adsorption of Metallic Ions
On examining toxic metallic ions, including lead, copper, cadmium, chrome, and barium, we found out that the title MOF can adsorb the former most effectively. This can be seen in Figure 6, in which Pb(II) ions are nearly 100% adsorbed, performing much better than the others.

Adsorption of Metallic Ions
On examining toxic metallic ions, including lead, copper, cadmium, chrome, and barium, we found out that the title MOF can adsorb the former most effectively. This can be seen in Figure 6, in which Pb(II) ions are nearly 100% adsorbed, performing much better than the others.

Desorption after Adsorption
After the adsorption of Pb(II), we tried to desorb it from the adsorbent to examine whether the structure of MOF remained or not. Primarily, we searched for lead ions, and, as shown in Figure 7, the Energy-Dispersive X-ray Spectroscopy (EDX). methods results illustrate the presence of the ions in the MOF after adsorption. Afterward, we desorb the ions by removing them from the MOF in D.I. water by washing them in RT three times,

Desorption after Adsorption
After the adsorption of Pb(II), we tried to desorb it from the adsorbent to examine whether the structure of MOF remained or not. Primarily, we searched for lead ions, and, as shown in Figure 7, the Energy-Dispersive X-ray Spectroscopy (EDX). methods results illustrate the presence of the ions in the MOF after adsorption. Afterward, we desorb the ions by removing them from the MOF in D.I. water by washing them in RT three times, then separating and drying the MOF. The XRD pattern of the empty MOF shown in Figure 8 illustrates some peaks similar to those of the initial MOF. This reveals that the MOF's structure has not been changed after the adsorption and desorption of lead ions. then separating and drying the MOF. The XRD pattern of the empty MOF shown in Figure 8 illustrates some peaks similar to those of the initial MOF. This reveals that the MOF's structure has not been changed after the adsorption and desorption of lead ions.

Conclusions
In this work, [Ca(H2btec)·H2O]n has been investigated for the absorption of heavy metals, and it has successfully absorbed about 96% of the Pb(II) in water after 15 min. It should be considered that the adsorbent has been synthesized using an environmentally friendly approach, and the aim was to absorb a pollutant that is very harmful to the environment. Therefore, this can be further researched using green chemistry. Finally, we found out that the MOF's structure remained after three times washes in an aqueous solution.  then separating and drying the MOF. The XRD pattern of the empty MOF shown Figure 8 illustrates some peaks similar to those of the initial MOF. This reveals that MOF's structure has not been changed after the adsorption and desorption of lead ion

Conclusions
In this work, [Ca(H2btec)·H2O]n has been investigated for the absorption of hea metals, and it has successfully absorbed about 96% of the Pb(II) in water after 15 min should be considered that the adsorbent has been synthesized using an environmenta friendly approach, and the aim was to absorb a pollutant that is very harmful to the vironment. Therefore, this can be further researched using green chemistry. Finally, found out that the MOF's structure remained after three times washes in an aqueo solution.
Author Contributions: M.A. and F.M. contributed equally to this manuscript. All authors h read and agreed to the published version of the manuscript.

Conclusions
In this work, [Ca(H 2 btec)·H 2 O] n has been investigated for the absorption of heavy metals, and it has successfully absorbed about 96% of the Pb(II) in water after 15 min. It should be considered that the adsorbent has been synthesized using an environmentally friendly approach, and the aim was to absorb a pollutant that is very harmful to the environment. Therefore, this can be further researched using green chemistry. Finally, we found out that the MOF's structure remained after three times washes in an aqueous solution.
Author Contributions: M.A. and F.M. contributed equally to this manuscript. All authors have read and agreed to the published version of the manuscript.